Fiber Reinforced Concrete (FRC) with Applications in Civil Engineering 2020
View this Special IssueResearch Article  Open Access
Juan Wang, Xun Li, Hongyuan Fang, Juan Zhang, Jinping Li, "Statistical Characteristics of Polymer Grouting Material Microstructure", Advances in Civil Engineering, vol. 2020, Article ID 8847494, 12 pages, 2020. https://doi.org/10.1155/2020/8847494
Statistical Characteristics of Polymer Grouting Material Microstructure
Abstract
The twocomponent foaming polyurethane is a kind of grouting material that has recently been widely used in engineering structural repair. Its physical and mechanical properties are closely related to its microstructure. Therefore, the qualitative and quantitative analysis of polymer microstructure has always been a research hotspot. The statistical characteristics of polymer grouting material microstructure are investigated by six groups of specimens with different densities, and the density varies from 0.1 to 0.6 g/cm^{3}. The microstructure morphology of polymer was observed and described by scanning electron microscopy (SEM), and the microstructure feature parameters were extracted and calculated by image processing technology. The quantitative analysis of section cell roundness distribution, cell diameter distribution, and polymer porosity shows that lowdensity polymer materials have anisotropy. While the density exceeds 0.3 g/cm^{3}, the cell structure tends to be spherical. The section cell diameters obey a normal distribution, and when the density increases, the cell diameter decreases. The porosity of the polymer has a linear negative correlation with the density. The polymer matrix has a density of 1.21 g/cm^{3}. The microstructural information obtained in this study will help establish a cellbased model to explain the mechanical response of rigid polymer foams.
1. Introduction
Nonwater reacted polymer grouting materials produced via a twocomponent polyurethane foam are a new kind of grouting materials [1]. Under grouting pressure, the polymer material reacts chemically, expands in volume, and rapidly solidifies [2]. This material has a good compressive strength [3], relatively high tensile strength [4], and good water impermeability [5]. It has been widely used in foundation reinforcement, void filling, antiseepage plugging, and other repair projects [6–9].
With the increase in engineering applications, the engineering properties of polymer grouting materials have also received extensive attention. In recent years, the research on the engineering properties of rigid polyurethane (RPU) has mainly focused on the relationship between material density, cellular microstructure, and physicomechanical properties. Hawkins et al. [10] studied the relationship between cell morphology, density, and mechanical properties in different positions of polyurethane samples with three mold sizes. The results showed that there is a relationship between cellular morphology and compression modulus and collapse stress in foamed plastics. And the shape and direction of cell not only affect the failure mechanism, but also affect the mechanical data. The authors of [11–14] studied the stressstrain behavior, microstructure characteristics, fatigue behaviour, and failure mode of RPU grouting materials under uniaxial compression, dynamic compression, and cyclic loading. Studies have shown that RPU grout materials with different densities show elastoplastic or atypical brittle characteristic; the main mechanical properties increase with increasing of density. In addition, the compressive failure of the material was caused by a yielding of the cell edges, and the manifestation of the microscopic fatigue failure was the expansion of the cracks in the cell walls and buckling of the cell edges. Ridha et al. [15] conducted experiments on the tensile properties of RPU materials, studied their microstructure characteristics, such as the size and geometric composition of the cells and struts, and defined the cell edges. The results showed that the cells were elongated under a tensile load; therefore, the material exhibited anisotropy, and the flexure of the struts at the cell edges were the main mechanism controlling the deformation and failure. Zheng et al. [16] conducted a study on RPU grouting materials through threepoint bending load and uniaxial compression tests and analyzed the mechanical behavior using a cell structure model. The results showed that the bending and compressive strengths of the polymer increased with the increase in density. In addition, with the increase in the density, the cell size decreased, and the degree of edge and corner polymerization between the cells decreased. Therefore, the antidamage ability of the cell was enhanced and the compression strength finally increased. Wu and He et al. [17, 18] studied the failure of RPU foam under a high temperature and vibration, and the degree of damage after treatment was evaluated through its tensile properties. The results showed that the tensile strength decreases with the increase in vibration amplitude and time, and the vibration failure of RPU foam was mainly due to the existence of microcracks in the cell structure. With the increasing heattreating temperature, the stress concentration in the RPU foam increased, and the tensile strength and modulus decreased due to the comprehensive effect of cell wall degradation and the generation of new defects.
The microimages of polyurethane polymers directly reflect many characteristics of the cellular structure. Through image analysis, many characteristics of the cell structure can be measured and characterized. According to the different image types, the image analysis and characterization methods of cell structure can be divided into 2D image analysis method and 3D image analysis method [19, 20]. The comparison between the two methods is shown in Table 1.

Twodimensional image analysis methods include microimage acquisition and computer image analysis methods. The 2D image of the cell structure is usually obtained by optical microscope (OM) [21–23] or scanning electron microscope (SEM) [24, 25]. The objective magnification of SEM can be changed from 10 times to more than 300,000 times. It can be used to detect small structural characteristics of foam, such as structural defects that damage the foam of samples [17, 18]. Computer image analysis method consists of image processing technology and image analysis technology [26]. Image processing technology corrects the blurring and other defects in the cell structure image and strengthens the cell information, so as to achieve the basic goal of correction and improvement of image quality. Image graying and threshold segmentation are common methods in 2D image processing. Computer image analysis technology refers to the extraction, description, and recognition of the characteristics (porosity, crosssection size, and crosssection shape of the cell) in the cell structure image based on a certain algorithm. However, the 2D image of cellular structure is a crosssection image of 3D structure, so the cell structure characteristics reflected in 2D images are not directly equivalent to the actual size of the feature in threedimensional space. Therefore, it is necessary to transform the features of 2D cell structure image into the actual 3D cell structure parameters according to the principles of solid geometry and statistics [27, 28].
In the same way, the 3D image analysis method needs to acquire the micro 3D structure image and carry out the computer 3D image processing. The 3D cell structure image needs to be obtained by 3D imaging methods, including optical tomography(OT) [29], laser confocal microscopy (LCM) [30], magnetic resonance imaging (MRI) [31, 32], Xray computerized tomography (XCT) [30, 33], and so on. On the basis of complex 3D image processing algorithm, threedimensional cell structure analysis and characterization of foam materials can be made by using a professional 3D image processing toolkit. Watershed segmentation and minimum intensity pixelizationbased method are two commonly used algorithms for computer 3D image processing [34, 35]. 3D images can reflect the cell morphology of foam plastics in three dimensions, and the cell structure information is much richer than 2D images. However, at present, this technology needs to be improved. The acquisition of 3D image is too expensive, and the processing is complex and timeconsuming, so it has not reached the stage of extensive practical application.
In this study, the microstructure of polymer grouting materials was observed and described by SEM, and the geometric characteristics of the size and shape of the cells under different densities were statistically analyzed with image processing technology. The quantitative relationship between geometric parameters such as cell content and size to polymer density are established. The purpose of this work is to provide a strategy for the research on the structure and performance of polymer grouting materials and suggest a potential method to study the mechanical properties and strength mechanism of polymer.
2. Statistics of Polymer Microstructure Characteristics
2.1. Test Overview
The twocomponent foaming polyurethane is primarily composed of polyols and isocyanates. The raw materials (Wanhua Energysav Science & Technology Group Co., Ltd., Yantai, Shandong, China) for the test are shown in Figure 1. Specimen casting, density measurement, and microstructure observation were carried out on the basis of the current standard GB/T 88132008 [36], GB/T 63432009 [37], and GB/T 128111991 [38]. The test mold adopts a split central cylinder with an inner diameter of 50 mm and a height of 600 mm, and the wall thickness is 10 mm. The onestep mechanical pouring foaming process was used. The two components, called white and black materials, were mixed evenly and quickly into the mold at room temperature (ambient temperature 15°C–20°C). After mixing, the two materials reacted violently and foamed rapidly, and the mold space was quickly filled. After 30 min, the specimen was removed from the mold after forming, and after standing for 3 h, the specimen was cut into a cylinder with a height of 100 mm. The weight of each specimen was taken and recorded, its actual density was calculated, and the specimens whose density met the requirements were numbered. To analyze the microstructure morphology and statistical characteristics of the polymer grouting materials, six groups of densities were designed, which were 0.1, 0.2, 0.3, 0.4, 0.5, and 0.6 g/cm^{3}. The measured densities were 0.11, 0.25, 0.31, 0.40, 0.51, and 0.56 g/cm^{3}, respectively.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
The microstructure of the polymer samples was observed by SEM. The samples used for the SEM test were processed as follows. A cylindrical core sample was taken along the center of the specimen with a core drilling machine (round drill bit, outer diameter 38 mm, inner diameter 2.8 mm) and then cut to a thickness of 20 mm on a machine tool. To improve its conductivity, the target section of the sample was sprayed with gold prior to the observation. A scanning electron microscope (KYKYEM6200, Beijing Zhongke Science and Technology Co., Ltd., Beijing, China) was used to observe the section of the sample, and structure images of the cells were taken.
2.2. Microstructure Feature Extraction
2.2.1. Microstructure Variables
The polymer grouting material has a kind of cell structure, whose internal feature parameters mainly include cell shape [34], cell size [39], cell size distribution [25], and cell content [10]. The parameters of roundness, cell diameter, and porosity are often used to measure the above geometric characteristics. The definition and calculation formula of each variable are as follows.(1)Section roundness (n) is the percentage of the ratio of 4π times the area to the perimeter square [27], represented in (1). The section roundness indicates the degree to which each cell section tends to be round. The percentage is closer to 100%, and the shape of the cell section is closer to be a circle; that is, when n = 100%, the cell section is circular. where c is the perimeter of the cell section, and s is the area of the cell section.(2)Section cell diameter (d) is the calculated size of a single cell in the crosssection. Each cell is equivalent to a circle, and the cell size is represented by the equivalent diameter of the circle. The length of the line segment passing through the centroid of the cell was measured every 2°, and then the average value, which is recorded as the cell diameter, is calculated. Section average cell diameter () is the arithmetic mean of all cell diameters in the statistical section, represented as In this formula, d_{i} is a possible value of the cell section diameter, and n_{i} is the number of cells with a cell diameter of d_{i}. Standard deviation of section cell diameter (S) is the distribution of the diameter of the cells in the statistical section, represented as where N is the total number of cells in the sample, d_{i} is the diameter of any cell section, and is the section average cell diameter. It is assumed that the cell is spherical and disordered. When the number of cells on the SEM image tends to infinity, there is also a quantitative relationship between the section average cell area and the average cell diameter. As shown in Figure 2, when a 2D image plane passes through a cell, the distance from the crosssection to the center of the cell is random, and the section area of the cell changes accordingly. When the number of cells passing through the twodimensional image plane is large, the average crosssectional area of cells () tends to a fixed value related to the cell diameter (D) [11], which is shown as follows: The cell diameter (D) can also be expressed by the average cell crosssectional area (): where A is the area of any cell section, x is the distance from the section to the cell center, and R is the cell diameter. The formula for calculating the standard deviation of cell diameter can be obtained by the differential equation (5): where S_{D} is the standard deviation of cell diameter and S_{A} is the standard deviation of the sectional area of the cell.(3)Porosity (f) is the ratio of the gas phase volume to the total volume, represented as
In this formula, is the volume of the gas phase, and is the total volume of the polymer.
It is difficult to directly measure the volume of the gas phase; therefore, the gas phase is determined according to the basic equation (8) of quantitative metallography [40].
In this formula, is the volume fraction of the measured phase, is the area fraction of the measured phase, and is the line segment fraction of the measured phase.
2.2.2. Analysis of the Structural Variables of Polymer Grouting Materials
Image processing technology was used to preprocess the SEM image. According to the definition of the microstructure variables, relevant geometric parameters in the image are extracted and the distribution characteristics are analyzed. The main steps are as follows.(1)Image preprocessing: The noncell information pixels on the picture are cut out, and the image with the largest size range is used. The size of the cropped image is approximately 4 mm × 4 mm, and each image can contain hundreds of cells, as shown in Figures 3(a) and 3(b).(2)Image reconstruction: Under the principle of image fidelity, the cells in the SEM image are filled with black by ImageJ software. Then, the filled SEM image is binarized to obtain black cells in a white background through MATLAB software, so that the target cells are highlighted (none of the above operations change the image pixel density). The reconstructed SEM image is shown in Figure 3(c).(3)Boundary processing: First, the incomplete cells at the edges of the picture are removed. Some of the cells in the material’s microstructure will be in contact with each other, and the smaller the density is, the more obvious this phenomenon is; therefore, the boundaries need to be processed. Based on the original image, the cells that touch each other are segmented by the Split Objects function of the ImagePro Plus software. The SEM image of the edge cell removal and the contact cell segmentation is shown in Figure 3(d).(4)Microstructure variable statistics: A pixel analysis is performed on the image obtained from steps 2 and 3 by the ImagePro Plus software. The porosity is obtained from the reconstructed image, and the other structural variable values are calculated from the removed and segmented image. All measured samples are counted, the microstructure variables of the polymers are calculated, and their distribution characteristics are analyzed.
3. Results and Discussion
3.1. Microstructure of Polymers
The formation of cells in polyurethane polymer materials is mainly described by the foaming process. Generally, the foaming process is divided into three stages: the nucleation of small bubbles in the liquid polymer, growth of small bubbles to a predetermined volume, and stabilization of the cell structure [24]. After curing, the polyurethane polymer material can be prepared. Figure 4 shows the microstructure of polymers with different magnification at different densities. Figures 4(a), 4(d), 4(g), 4(j), 4(m), and 4(p) are SEM images of the polyurethane polymer materials at approximately 20 times magnification for six groups of densities. It can be seen that, on the microscopic scale, the material is composed of closely contacted and closed cells. The difference in the material density is mainly due to the structural characteristics of the cells, except for the density of the polymer matrix material. As the density increases, the shapes of the polymer cells tend to change from polygons to ellipses and circles, the cell diameter decreases, the cell spacing increases, and the porosity decreases.
(a)
(b)
(c)
(d)
(e)
(f)
(g)
(h)
(i)
(j)
(k)
(l)
(m)
(n)
(o)
(p)
(q)
(r)
For 0.11 g/cm^{3} SEM image, in Figure 4(b) (magnified 100 times), the cell diameter is generally greater than 150 μm, the cell structure is irregular and nonuniform, and the cell crosssection is generally hexagonal. The contact surface (face) between each cell is large, and the faces with a thin film means that the cells have a high closed cell ratio. The strut is between two adjacent faces. The vertex is at strut intersection. Most of the matrix material is concentrated on the struts and vertices that make up the cell frame. In Figure 4(c) (magnified 200 times), the faces are generally greater than 50 μm, and the face shape is oval. There are usually twelve faces in the cell, which means that the cell is a dodecahedron. There are many triangle cut struts, and the struts are long and thin. It can be seen that struts play a major supporting role. Under load, struts will buckle and faces will crack [13].
For 0.25 g/cm^{3} SEM image, in Figure 4(e) (magnified 100 times), the cell diameter is generally greater than 120 μm, and the cell structure is an ellipse with large ellipticity. The number of intracellular faces slightly decreased, and the face is relatively large. In Figure 4(f) (magnified 200 times), the faces are generally greater than 40 μm, and the face shape is round or oval. The number of intracellular faces decreased. The struts become thicker and shorter, and the triangle cut strut reduction.
For 0.31 g/cm^{3} SEM image, in Figure 4(h) (magnified 100 times), the cell diameter is generally less than 260 μm, and the cell shape is circular or elliptical. The face is relatively small. The cells basically meet the closest packing. In Figure 4(i) (magnified 200 times), the faces are usually less than 50 μm, and the shape of the face tends to be circular. The number of triangle cut struts further reduces, the polygonal cut strut increases, and the length of strut is reduced.
For 0.40 g/cm^{3} SEM image, in Figure 4(k) (magnified 100 times), the cell diameter is generally less than 220 μm, and the cell shape is an ellipse with very small ellipticity. Some adjacent cells do not contact each other and there are a lot of matrix materials between them, and the number of face further reduced. In Figure 4(l) (magnified 200 times), the faces are usually less than 40 μm, and the faces are with a thin film. The part of the adjacent triangular cut struts merges, and the struts are wide and short.
For 0.51 g/cm^{3} SEM image, in Figure 4(n) (magnified 100 times), the cell diameter of the specimen is generally less than 180 μm, and the cell shape is round or oval with a small ellipticity. The face is extremely small. The matrix material of adjacent cells increased. In Figure 4(o) (magnified 200 times), the faces are usually less than 30 μm, and the number of intracellular faces decreased significantly. The cut strut of triangle is obviously reduced.
For 0.56 g/cm^{3} SEM image, in Figure 4(q) (magnified 100 times), the cell diameter of the specimen is generally less than 150 μm, and the cell shape is basically round. There are almost no windows mean cells do not touch. There are a lot of matrix materials between cells. In Figure 4(r) (magnified 200 times), the faces are usually less than 20 μm. There are almost no triangle cut struts. It can be seen that the strength of polymer increases with the increase of matrix material content and cell spacing [16].
3.2. Statistical Analysis of the Polymer Cell Geometry
By observing the SEM morphology of the polyurethane polymer material, an intuitive understanding of the cell structure of the polymer is obtained, which provides a basis for determining the geometric characteristics of the cell. The statistical results of the roundness distribution, cell diameter distribution, and porosity are as follows.
3.2.1. Section Roundness Distribution
Figure 5 is a section cell roundness distribution diagram for polyurethane polymer samples of each density. It can be seen from Figure 4 that, for lowdensity materials, the section cells with a roundness between 90% and 100% account for only 50% to 70% of the total cells, and there are a few cells with a section roundness less than 75%. The reason for this phenomenon is that the cells squeeze each other due to the increase in cell diameter, and the shape tends to be an ellipsoid or an irregular polyhedron. When the density of the polymer is higher than 0.3 g/cm^{3}, the proportion of cells with a section roundness of 90% to 100% is higher than 80%, and the section roundness of most of the cells is higher than 75%. Therefore, with the increase in density, the shape of the polymer cells tends to be round.
As shown in Table 2, the statistical parameters of the section roundness of the cells at each density is further calculated. It can be seen that as the density of the polymer increases, the average value of the section roundness of the cells increases. By comparing the average values and median of the section roundness at each density, it can be seen that the anisotropy of the cells in the specimen is not serious, especially that the highdensity specimen is basically close to the ball, which may be related to the location of the sample in the specimen [10], so it is appropriate to use the average sphere size to characterize the cell size in (4). When the density exceeds 0.3 g/cm^{3}, the section roundness of the cells approaches 100%, and this result indicates that the shape of the cells is closer to a sphere, and the macroscopic performance is close to isotropic.

3.2.2. Cell Diameter Distribution
Figure 6 is a section cell diameter distribution chart for the polyurethane polymer specimens with different densities. It can be seen from Figures 6(a)–6(f) that the section cell diameter distribution of each density specimen basically follows the normal distribution. As the density of the specimen increases, the length and endpoint of the section cell diameter distribution interval decreases. Figure 7 shows a summary of the section cell diameter distribution. It can be seen from Figure 7 that as the density of the specimen increases, the overall size of the section cell diameter decreases, and the degree of dispersion of the section cell diameter distribution also decreases. And the average section cell diameter and standard deviation of the specimens at each density are negatively correlated with the density.
(a)
(b)
(c)
(d)
(e)
(f)
As shown in Table 3, the statistical parameters of the section cell diameter distribution of the cells at each density is further calculated. With the increase of density, the statistical parameters tend to decrease.

According to (5), the average section cell area measured by the computer twodimensional image analysis software ImagePro Plus is transformed into the cell diameter. According to (6), the standard deviation of the cell crosssection area is converted into the standard deviation of the cell diameter. In this way, the measured twodimensional area can be transformed from SEM image to threedimensional cell diameter and distribution. The average cell diameter, standard deviation, and density of the polymer materials were fitted, and it is found that they have a basically linear relationship. Figure 8 is a fitting graph of each cell diameter parameter and density.
(a)
(b)
As shown in Figure 8(a), a linear fitting of the average cell diameter and density can be obtained as follows:where D is the average cell diameter, and is the polymer density.
As shown in Figure 8(b), a linear fitting of the standard deviation and density of the cell diameter distribution can be obtained as follows:where S_{D} is the standard deviation of the cell diameter distribution, and is the polymer density.
The quantification of cell size is helpful to understand the influence of microstructure on the mechanical properties of materials. When the cell size is large, the compressive property of the material is mainly determined by the strut. According to the previous studies, the critical cell size of the turning point which defines the influence of cell size on compressive strength increases with the increase of density. The results show that the cell size of 0.60 g/cm^{3} specimen is more than 60 μm, which is larger than the critical cell size [41]. Therefore, it can be inferred that the compression failure of materials is caused by the yielding of struts [11].
3.2.3. Polymer Porosity
The density of the polyurethane polymer material is obviously related to the polymer porosity and density of the matrix. As shown in Figure 9, as the density increases, the polymer porosity decreases.
A linear fit of the porosity and density of the polymer yields the following relationship:
In this formula, f is the porosity, and is the polymer density.
According to (11), when the porosity is 0, the polymer matrix density is 1.21 g/cm^{3}. It is basically consistent with the description in literature [42] that the matrix density of rigid polyurethane foam is about 1.2 g/cm^{3}.
4. Conclusions
In this study, micromorphology SEM images of the specimens were observed, and feature parameters were counted. The microstructural information obtained in this study will help establish a cellbased model to explain the mechanical response of rigid polymer foams. The main results and conclusions are as follows:(1)The cells of the lowdensity polymer material are deformed due to the mutual extrusion of the cells, which are irregular polyhedrons or ellipsoids. Therefore, lowdensity polymer materials have anisotropy. As the density increases and exceeds 0.3 g/cm^{3}, the cell structure tends to be spherical, and the polymer materials are close to isotropic.(2)The section cell diameters in the same specimen obey a normal distribution, and the section average cell diameter, standard deviation, the length and endpoint of the section cell diameter distribution interval decrease as the density of the specimen increases. The cell diameter and standard deviation have linear negative correlations with the density.(3)The porosity of the polymer has a linear negative correlation with the density. The polymer matrix has a density of 1.21 g/cm^{3}.
Data Availability
The data used in the paper are available from the authors upon request.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
The authors would like to acknowledge the financial support received from the National Key Research and Development Program of China (no. 2018YFC1508401) and the Open Fund Project of State Key Laboratory of Road Engineering Safety and Health in Cold and HighAltitude Regions of China (no. YGY2017KYPT03).
References
 H. Liu, F. Wang, M. Shi, and W. Tian, “Mechanical behavior of polyurethane polymer materials under triaxial cyclic loading: a particle flow code approach,” Journal of Wuhan University of Technology, vol. 33, no. 4, pp. 980–986, 2018. View at: Publisher Site  Google Scholar
 M. Hao, F. Wang, X. Li, B. Zhang, and Y. Zhong, “Numerical and experimental studies of diffusion law of grouting with expansible polymer,” Journal of Materials in Civil Engineering, vol. 30, no. 2, 2018. View at: Publisher Site  Google Scholar
 M. Shi, F. Wang, and J. Luo, “Compressive strength of polymer grouting material at different temperatures,” Journal of Wuhan University of Technology, vol. 25, no. 6, pp. 962–965, 2010. View at: Publisher Site  Google Scholar
 M. Shi, “Research on polymer grouting material properties and directional fracturing grouting mechanism for dykes and dams,” Dalian University of Technology, Dalian, China, 2010, PhD Thesis. View at: Google Scholar
 N. Rana and R. Nair, “Performance of polyurethane grouting to handle heavy seepage in tunnels,” in Proceedings of the Conference on Recent Advances in Rock Engineering (RARE), Bengaluru, India, 2016. View at: Google Scholar
 O. Buzzi, S. Fityus, Y. Sasaki, and S. Sloan, “Structure and properties of expanding polyurethane foam in the context of foundation remediation in expansive soil,” Mechanics of Materials, vol. 40, no. 12, pp. 1012–1021, 2008. View at: Publisher Site  Google Scholar
 H. Fang, B. Li, F. Wang, Y. Wang, and C. Cui, “The mechanical behaviour of drainage pipeline under traffic load before and after polymer grouting trenchless repairing,” Tunnelling and Underground Space Technology, vol. 74, pp. 185–194, 2018. View at: Publisher Site  Google Scholar
 H. Fang, Y. Su, X. Du, F. Wang, and B. Li, “Experimental and numerical investigation on repairing effect of polymer grouting for settlement of highspeed railway unballasted track,” Applied Sciences, vol. 9, p. 21, 2019. View at: Publisher Site  Google Scholar
 C. Guo, B. Sun, D. Hu, F. Wang, M. Shi, and X. Li, “A field experimental study on the diffusion behavior of expanding polymer grouting material in soil,” Soil Mechanics and Foundation Engineering, vol. 56, no. 3, pp. 171–177, 2019. View at: Publisher Site  Google Scholar
 M. C. Hawkins, B. O’Toole, and D. Jackovich, “Cell morphology and mechanical properties of rigid polyurethane foam,” Journal of Cellular Plastics, vol. 41, no. 3, pp. 267–285, 2005. View at: Publisher Site  Google Scholar
 Y. Wei, F. Wang, X. Gao, and Y. Zhong, “Microstructure and fatigue performance of polyurethane grout materials under compression,” Journal of Materials in Civil Engineering, vol. 29, no. 9, 2017. View at: Publisher Site  Google Scholar
 L. Shi and Z.M. Li, “Morphology development of highdensity rigid polyurethane foam upon compression by online scanning electronic microscope,” Journal of Applied Polymer Science, vol. 105, no. 4, pp. 2008–2011, 2007. View at: Publisher Site  Google Scholar
 K. Liu, W. Liang, F. Ren, J. Ren, F. Wang, and H. Ding, “The study on compressive mechanical properties of rigid polyurethane grout materials with different densities,” Construction and Building Materials, vol. 206, pp. 270–278, 2019. View at: Publisher Site  Google Scholar
 E. Linul, D. A. Şerban, L. Marsavina, and T. Sadowski, “Assessment of collapse diagrams of rigid polyurethane foams under dynamic loading conditions,” Archives of Civil and Mechanical Engineering, vol. 17, no. 3, pp. 457–466, 2017. View at: Publisher Site  Google Scholar
 M. Ridha and V. P. W. Shim, “Microstructure and tensile mechanical properties of anisotropic rigid polyurethane foam,” Experimental Mechanics, vol. 48, no. 6, pp. 763–776, 2008. View at: Publisher Site  Google Scholar
 X. Zheng, “Study on relationship between density and mechanical behavior of high polymer grouting materials,” Journal of Wuhan University of Technology, vol. 36, no. 4, pp. 44–47, 2014. View at: Publisher Site  Google Scholar
 J. Wu, Y. He, and Z. Yu, “Failure mechanism of rigid polyurethane foam under high temperature vibration condition by experimental and finite element method,” Journal of Applied Polymer Science, vol. 137, no. 6, 2019. View at: Publisher Site  Google Scholar
 Y. He, J. Wu, D. Qiu, and Z. Yu, “Experimental and numerical analyses of thermal failure of rigid polyurethane foam,” Materials Chemistry and Physics, vol. 233, pp. 378–389, 2019. View at: Publisher Site  Google Scholar
 K. Mader, R. Mokso, C. Raufaste et al., “Quantitative 3D characterization of cellular materials: segmentation and morphology of foam,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 415, pp. 230–238, 2012. View at: Publisher Site  Google Scholar
 S. PérezTamarit, E. Solórzano, A. Hilger, I. Manke, and M. A. RodríguezPérez, “Multiscale tomographic analysis of polymeric foams: a detailed study of the cellular structure,” European Polymer Journal, vol. 109, pp. 169–178, 2018. View at: Publisher Site  Google Scholar
 Z. Zakaria, Z. Mohamad Ariff, and A. Abu Bakar, “Monitoring deformation mechanism of foam cells in polyethylene foams via optical microscopy: effect of density and microstructure,” Journal of Cellular Plastics, vol. 54, no. 6, pp. 957–976, 2018. View at: Publisher Site  Google Scholar
 C. Yang, Z.H. Zhuang, and Z.G. Yang, “Pulverized polyurethane foam particles reinforced rigid polyurethane foam and phenolic foam,” Journal of Applied Polymer Science, vol. 131, no. 1, 2014. View at: Publisher Site  Google Scholar
 E. Esmaeilnezhad, M. Rezaei, and M. K. Razavi, “The effect of alternative blowing agents on microstructure and mechanical characteristics of rigid polyurethane foam,” Iranian Polymer Journal, vol. 18, no. 7, pp. 569–579, 2009. View at: Publisher Site  Google Scholar
 J. R. Dawson and J. B. Shortall, “The microstructure of rigid polyurethane foams,” Journal of Materials Science, vol. 17, no. 1, pp. 220–224, 1982. View at: Publisher Site  Google Scholar
 J. Reignier, P. Alcouffe, F. Mechin, and F. Fenouillot, “The morphology of rigid polyurethane foam matrix and its evolution with time during foaming  new insight by cryogenic scanning electron microscopy,” Journal of Colloid and Interface Science, vol. 552, pp. 153–165, 2019. View at: Publisher Site  Google Scholar
 J. Pinto, E. Solórzano, M. A. RodriguezPerez, and J. A. de Saja, “Characterization of the cellular structure based on userinteractive image analysis procedures,” Journal of Cellular Plastics, vol. 49, no. 6, pp. 555–575, 2013. View at: Publisher Site  Google Scholar
 K. M. Lewis, I. Kijak, K. B. Reuter, and J. B. Szabat, “An image analysis method for cellsize and cellsize distribution measurement in rigid foams,” Journal of Cellular Plastics, vol. 32, no. 3, pp. 235–259, 1996. View at: Publisher Site  Google Scholar
 D. L. Sahagian and A. A. Proussevitch, “3D particle size distributions from 2D observations: stereology for natural applications,” Journal of Volcanology and Geothermal Research, vol. 84, no. 3, pp. 173–196, 1998. View at: Publisher Site  Google Scholar
 R. GarciaGonzales, C. Monnereau, J. F. Thovert, P. M. Adler, and M. VignersAdler, “Conductivity of real foams,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 151, no. 3, pp. 497–503, 1999. View at: Publisher Site  Google Scholar
 F. De Pascalis, M. Nacucchi, M. Scatto, and R. Albertoni, “Quantitative characterisation of lowdensity, high performance polymeric foams using high resolution Xray computed tomography and laser confocal microscopy,” NDT & E International, vol. 83, pp. 123–133, 2016. View at: Publisher Site  Google Scholar
 G. Ovarlez, K. Krishan, and S. CohenAddad, “Investigation of shear banding in threedimensional foams,” Europhysics Letters, vol. 91, no. 6, Article ID 68005, 2010. View at: Publisher Site  Google Scholar
 J. Braun, M. O. Klein, J. Bernarding, M. B. Leitner, and H. D. Mika, “Nondestructive, threedimensional monitoring of water absorption in polyurethane foams using magnetic resonance imaging,” Polymer Testing, vol. 22, no. 7, pp. 761–767, 2003. View at: Publisher Site  Google Scholar
 M. MarviMashhadi, C. S. Lopes, and J. Llorca, “Modelling of the mechanical behavior of polyurethane foams by means of micromechanical characterization and computational homogenization,” International Journal of Solids and Structures, vol. 146, pp. 154–166, 2018. View at: Publisher Site  Google Scholar
 M. D. Montminy, “Complete structural characterization of foam using 3D images,” University of Minnesota, Ann Arbor, MI, USA, 2001, PhD Thesis. View at: Google Scholar
 M. D. Montminy, A. R. Tannenbaum, and C. W. Macosko, “The 3D structure of real polymer foams,” Journal of Colloid and Interface Science, vol. 280, no. 1, pp. 202–211, 2004. View at: Publisher Site  Google Scholar
 General Administration of Quality Supervision, “Inspection and quarantine of the People’s Republic of China, standardization administration of the People’s Republic of China,” Rigid Cellular PlasticsDetermination of Compression Properties, Standards Press of China, China, 2008. View at: Google Scholar
 General Administration of Quality Supervision, “Inspection and quarantine of the People’s Republic of China and standardization administration of the People’s Republic of China,” Cellular Plastics and RubbersDetermination of Apparent Density, Standards Press of China, China, 2009. View at: Google Scholar
 General Administration of Quality Supervision, “Inspection and quarantine of the People’s Republic of China,” Test Method for Average Cell Size of Rigid Cellular Plastics, Standards Press of China, China, 1991. View at: Google Scholar
 J. Xu, T. Wu, J. W. Zhang, H. Chen, W. Sun, and C. Peng, “Microstructure measurement and microgeometric Packing characterization of rigid polyurethane foam defects,” Cellular Polymers, vol. 36, no. 4, pp. 183–204, 2017. View at: Publisher Site  Google Scholar
 M. B. Rhodes and B. Khaykin, “Foam characterization and quantitative stereology,” Langmuir, vol. 2, no. 5, pp. 643–649, 1986. View at: Publisher Site  Google Scholar
 G. F. Smits, “Effect of cellsize reduction on polyurethane foam physical properties,” Journal of Thermal Insulation and Building Envelopes, vol. 17, no. 4, pp. 309–329, 1994. View at: Publisher Site  Google Scholar
 L. J. Gibson and M. F. Ashby, “The mechanics of threedimensional cellular materials,” Proceedings of the Royal Society of London. A. Mathematical and Physical Sciences, vol. 382, no. 1782, pp. 43–59, 1982. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2020 Juan Wang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.